The effect of carboxylate position on the structure of a metal organic framework derived from cyclotriveratrylene †

Two cyclotriveratrylene-based ligands H 3 L 1 and H 3 L 2 have been synthesised using microwave heating and used in the formation of 1 [Zn 2 ( L 1 )(DMA) 2 (CH 3 COO)] and 2 [Zn 6 ( L 2 ) 4 (DMA) 6 (H 2 O) 5 ] (DMA = N , N -dimethylacetamide). 1 displays an unusual trigonal paddlewheel node geometry, while Zn( II ) paddlewheels are observed in 2 . However, the stacking of CTV molecules in 1 is replaced by an uncommon molecular capsule structure in 2 .


Introduction
Controlling self-assembly in the solid state is one of the major goals of crystal engineering.2][3][4][5] Of these, ligand substitution or alteration can result in dramatically different structures under the same conditions of self-assembly.Specifically, the position of a substituent on an aromatic substrate can result in significantly different properties of the resultant compounds, with perhaps the best example of this being the xylenes, where the position of the methyl groups on the benzene ring gives differences in boiling point, viscosity and crystal structure. 6ne area where systematic substitution of functional groups is hugely important is that of supramolecular self-assembly, in which complex structure and function arise during materials synthesis from often delicately balanced structural and electronic factors. 7This approach is particularly common in the synthesis of coordination polymers and the asso-ciated sub-discipline of metal organic frameworks (MOFs).][10][11][12][13] Here, a change in the position of a functional group such as a carboxylate can result in a completely different structure as a result of the changed connectivity of the organic linker.This has been observed for numerous linkers, ranging from simple substrates such as benzoic or pyridinecarboxylic acids [14][15][16][17] to more complex molecules such as porphyrinic macrocycles. 18,19acrocycles such as porphyrins, 20 calixarenes, 21 crown ethers 22,23 and cyclodextrins 24 have been used as ligands for the formation of MOFs.However, due to the increased complexity associated with such substrates, this is a relatively underexplored area.The use of macrocycles as linkers offers advantages such as a higher density of functional sites per molecule and additional coordination sites such as hydrophobic pockets or ion binding regions, when compared to simpler substrates.Cyclotriveratrylenes (CTVs) are one such class of bowl-shaped macrocycles containing a shallow, hydrophobic pocket and an upper rim which can be functionalised in a number of ways. 259][30][31][32][33] A few examples of coordination polymers based upon CTVs have also been reported, including low dimensional coordination polymers with lanthanide ions, 33 a covalent organic framework (COF) based upon a triformyl CTV derivative 34 and a MOF featuring one of the ligands used in this study, (L 1 ) 3− , coordinated to a copper node, giving rectangular one-dimensional pores. 35ere, we report the synthesis of the linkers H 3 L 1 and This journal is © The Royal Society of Chemistry 2017 using a microwave Suzuki coupling procedure, we are able to achieve greater yields and shorter reaction times than those previously reported for Suzuki couplings involving CTVs as a substrate. 36We have used these linkers in solvothermal reactions and confirm that the structures of the materials obtained are strongly dependent on the position of the carboxylate.For the para benzoic acid-substituted H 3 L 1 , a columnar stacking of CTV molecules is observed.However, the change in directionality provided by the meta benzoic acid component in H 3 L 2 results in the formation of a molecular capsule arrangement which has not been observed previously for coordination polymers.

Experimental section
Tribromocyclotriveratrylene (CTV-Br 3 ) was prepared from 3-hydroxybenzoic acid in 15% yield according to a literature procedure, 37 and this compound was used as the substrate for Suzuki couplings.Couplings were performed under an inert atmosphere using a microwave reactor at 100 °C for 30 min, with 5 mol% PdĲPPh 3 ) 4 as catalyst with cesium fluoride and six equivalents of x-ethoxycarbonylphenylboronic acid (x = 4 for H 3 L 1 , 3 for H 3 L 2 ).Following purification and hydrolysis of the ester groups (full experimental details can be found in the ESI †), H 3 L 1 and H 3 L 2 were obtained as racemic mixtures in 75% and 58% yield, respectively (Scheme 1).
The complex 1-Zn was obtained by solvothermal reaction of H 3 L 1 with Zn(NO 3 ) 2 •6H 2 O in a solvent mixture of N,Ndimethylacetamide (DMA) and ethanol (2.5 : 1) in the presence of acetic acid at 90 °C.Upon cooling and filtration, colourless needles suitable for X-ray diffraction analysis were obtained.1 was obtained as isostructural cobalt(II) and zinc(II) complexes, 1-Zn and 1-Co, respectively.However only 1-Zn will be discussed here in detail.2-Zn was synthesised in a similar manner but in the absence of acetic acid, where after cooling and filtration, colourless hexagonal plates of suitable quality were obtained for X-ray diffraction studies.The addition of acetic acid to this second solvothermal reaction mixture resulted in no crystalline material being produced.addition to a bidentate acetate molecule (Fig. 1b).Together, this arrangement of metal centres can be thought of as an asymmetric trigonal paddlewheel, where on one side, in addition to an axial solvent (in this case DMA) molecule, there is bidentate coordination to an acetate.Trigonal paddlewheel structures are uncommon, [38][39][40] and this is the first example of a metal organic framework containing a metal node bearing this trigonal paddlewheel geometry.

Results and discussion
The molecules of [L 1 ] 3− stack in a columnar arrangement, with a distance of 4.9 Å between hydrophobic CTV pockets.This motif is commonly observed in crystal structures of molecular CTV-based species, [28][29][30] presumably because it maximises the π-π interactions between CTV cores.In the columnar arrangement in this structure, left and right handed molecules of [L 1 ] 3− stack alternately.This reduces any steric hindrance associated with extending the CTV cores through the addition of the benzoic acid moiety.
When viewed down the b axis, three types of channels are visible: a rhombic channel (8.65 × 9.97 Å), a pentagonal channel (5.68 (pentagon base width) × 12.63 (width of channel at its widest point) × 13.43 (channel height) Å) and a hexagonal channel (12.30 × 13.89 Å) (Fig. 1c).The rhombic channel is occupied by two solvent molecules and the pentagonal channel by two solvent molecules and two acetate molecules, but the hexagonal channel remains free of any coordinated solvents.Using a 1.2 Å probe, the solvent accessible volume for this structure is calculated to be 5.5% using the Mercury program from the CCDC software package, 41 which is solely due to the unoccupied hexagonal pores.During this calculation, metal coordinated solvent molecules were not removed.When viewed down the b axis, a hexagonal superstructure composed of four of each type of channel is visible, with each side being approximately 22 Å (Fig. 1d).
Compound A capsular arrangement of CTVs in the solid state is uncommon, and although some examples have been shown for cyclotricatechylene (CTC), 42,43 the only examples reported for CTV-based structures incorporate complementary binding groups at their upper rim. 44,45In this structure, each molecular capsule is composed of one left handed and one right handed [L 2 ] 3− ligand, and when viewed down the c axis it can be seen that these capsules pack into a hexagonal arrangement (Fig. 2b), with one molecular capsule positioned at each corner of the hexagon.These hexagons stack in an alternating abab manner, which reduces the available porosity for this structure.However, the solvent accessible volume was calculated to be 21%, which is markedly higher than that for 1-Zn (which is 5.5%)This is due to the presence of two types of rectangular pores in 2-Zn of dimensions 7.57 × 6.28 Å and 12.55 × 10.57Å (Fig. 2c), as well as the interior of the capsules.
It can be seen that in the structures of 1-Zn and 2-Zn there is a balance between the preferred ligand geometry for the CTV ligand.In 1-Zn the CTV molecules stack on top of one another to maximise π-π interactions, with a preferred metal node geometry incorporating a trigonal ZnĲII) paddlewheel.][48] For the case of the para benzoic acid appended CTV, [L 1 ] 3− , the stacking interactions between CTV molecules are more favoured than the formation of four-blade ZnĲII) paddlewheels.This results in the formation of an unusual trigonal paddlewheel metal node, where each ZnĲII) cation in the paddlewheel has a different coordination number.This is in contrast to the previously reported MOF using this ligand, 35 where [L 1 ] 3− is connected through CuĲII) paddlewheels (where the copper displays octahedral coordination) and a five-coordinate, square bipyramidal CuĲII) to form rectangular, one dimensional nanotubes.In that structure, no stacking of the CTV molecules is observed.
For 2-Zn, the formation of the four-blade ZnĲII) paddlewheel structure is more favoured, resulting in an uncommon molecular capsule arrangement for the meta benzoic acid appended CTV, which results in a higher level This journal is © The Royal Society of Chemistry 2017 of porosity.As the reaction conditions in both cases are almost identical, it must be concluded that it is the position of the carboxylic acid which plays the major role determining the structural outcome of the synthesis.

Conclusions
In this work we have synthesised the para and meta benzoic acid appended cyclotriveratrylenes H 3 L 1 and H 3 L 2 , respectively, through a microwave assisted Suzuki coupling reaction.The use of microwave irradiation affords markedly faster reaction times and greater yields when compared with previously reported syntheses.We then used these ligands in solvothermal reactions with Zn(NO 3 ) 2 to give the corresponding coordination polymers 1-Zn and 2-Zn.For both of these frameworks, it can be seen that there is a finely balanced compromise between optimal ligand packing and metal node geometry.For 1, the common CTV packing motif is observed where CTV molecules stack on top of one another, which results in an unusual trigonal paddlewheel metal node geometry.For 2-Zn, the common four-blade paddlewheel geometry is seen, although this yields an uncommon molecular capsule arrangement of the CTV ligand.Thus, we have confirmed that the position of the carboxylic acid, here meta or para, plays a critical role in the assembly of CTV-based MOFs.This is important for the future design of porous materials based upon macrocyclic scaffolds, where maintaining porosity and functionality is crucial.

Fig. 1
Fig. 1 View of the asymmetric unit of 1 (a), metal node geometry of 1 displaying a trigonal paddlewheel (b), three different types of channels in 1 as viewed down the b axis (c), and hexagonal superstructure of channels outlined in red (d).Hydrogen atoms in b-d have been omitted for clarity.

2 -
Zn crystallises in the triclinic space group P1 ¯, with the asymmetric unit containing four molecules of [L 2 ] 3− , six ZnĲII) cations, six molecules of DMA and five water molecules (Fig. 2a), thus yielding a product of formula [Zn 6 (L 2 ) 4 (DMA) 6 (H 2 O) 5 ].Unlike the reaction with [L 1 ] 3− , in the presence of acetic acid the reaction of [L 2 ] 3− with Zn(II) af-fords no crystalline material in our hands.The arrangement of the CTV ligands in 2-Zn is distinctly different to that observed in 1-Zn; a molecular capsule arrangement of [L 2 ] 3− ligands is observed in 2-Zn, with no stacking interactions observed between CTV ligands in this structure.The molecular capsules are connected to each other through four-blade Zn(II) paddlewheels, as opposed to the trigonal paddlewheel structure observed for 1-Zn.The zinc paddlewheels are axially coordinated by one water molecule and one DMA molecule, with two unbound DMA molecules found inside each molecular capsule, and one addition DMA molecule exo to the capsules.

Fig. 2
Fig. 2 View of the asymmetric unit of 2 (a), hexagonal arrangement of molecular capsules as viewed down the c axis (b) and two types of rectangular pores in the structure as viewed down the a axis (c).Hydrogen atoms and uncoordinated solvent molecules in b and c have been removed for clarity.
in which a cyclotriveratrylene scaffold is functionalised with para and meta-benzoic acid group, respectively.Notably, d School of Chemistry, University of Manchester, Oxford Road, Manchester, M13 9PL, UK.E-mail: M.Schroder@manchester.ac.uk † Electronic supplementary information (ESI) available.CCDC 1470195-1470197.For ESI and crystallographic data in CIF or other electronic format see DOI: 10.1039/c6ce01965j